Spreadsheet: 2356dacc-60fb-41cd-9075-114092c0521a
Sheet: 11. Pipe

 |  |  |  |  | MD-SLS; Part of SOP
M-spec |  | Linked standards |  | Material / Grade | Dimension limitation | Product | Certificate |  | Delivered condition |  | Chemical composition |  |  |  |  |  |  | Yield & Tensile |  |  |  |  |  |  |  |  |  | Impact energy |  |  |  | Hardness (maxim) |  | Supplementary requirements | [NAME] Testing | Added tests
 |  | NORSOK | Other |  |  |  |  | Production method | Heat treatment | Temp minimum | Cast / Ladle analysis |  | Product analysis |  | CEV | IIW | Pcm | Minimum yield strength |  |  | [NAME] strength |  |  | Ratio | Elongation (minimum) |  |  | Temp | Sample thickn. | Energy J
 | rev. |  |  |  | m m |  |  |  |  | ºC | Element | Content % | Element | Content % |  |  |  | Dimension mm | KSI | MPa | Dimension mm | KSI | MPa | % | Dimension mm | % | Reduction of area | ºC | m m | average | single | Test material | Forging surface
M10020 | C | Modified M630, MDS C22,  rev 4 | API 5L | X-65  PSL 2 |  | Seamless pipe | EN 10204 3.1 shall include the following information: - Melting and refining practice, - Heat treatment conditions (For QT condition austenitisation and tempering temperature and quenching medium shall be stated.) |  | Normalized or Quenched and Tempered | x | C Mn P S Si  Al Ti Nb V+Nb+Ti V+Nb N | [NAME] 0.16 0.90 - 1.60 max 0.035 [NAME] 0.025 0.10 - 0.50 max 0.06 max 0.05 [NAME] 0.04 max 0.12 max 0.10 max 0.015 |  |  | 0.43 |  |  |  | 65 - 87 | 448 - 600 |  | 77 - 110 | 531 - 758 | 0.93 |  | x |  | -46 | t>6mm  Reduction factors for subsize specimens shall be:  7.5 mm - 5/6  5 mm - 2/3. | 45 | 38 | 237 HBW |  |  | 100 UT
M10020 | B | Modified M630, MDS C22,  rev 4 | API 5L | X-65  PSL 2 |  | Seamless pipe | EN 10204 3.1 shall include the following information: - Melting and refining practice, - Heat treatment conditions (For QT condition austenitisation and tempering temperature and quenching medium shall be stated.) |  | Normalized or Quenched and Tempered | x | C Mn P S Si  Al Ti Nb V+Nb+Ti V+Nb N | [NAME] 0.16 0.90 - 1.60 max 0.035 [NAME] 0.025 0.10 - 0.50 max 0.06 max 0.05 [NAME] 0.04 max 0.12 max 0.10 max 0.015 |  |  | 0.43 |  |  |  | 65 - 87 | 448 - 600 |  | 77 - 110 | 531 - 758 | 0.93 |  | x |  | -46 | t>6mm  Reduction factors for subsize specimens shall be:  7.5 mm - 5/6  5 mm - 2/3. | 45 | 38 | 237 HB
M10168 | D |  | ISO 3183:2007 / API 5L 44th edition  ISO 15156-2 / NACE MR 01-75  ASTM A370 ASTM E10 ASTM E23 ASTM E112 ASTM E114 ASTM E 1823  ISO 6507-1 / ASTM E 92 ISO 6508 / ASTM E 18 ISO 8501-1 ISO 9303 / ASTM E213  ISO 10124 NB: Superseded by: ISO 10893-8  ISO 10543 NB: Superseded by: ISO 10893-12  ISO 15156 | API 5L  Carbon steel  X70 C-Mn  PSL2 |  | Seamless pipe Manifold piping Jumpers Spools | EN 10204 Type 3.1 + BP approved 3rd party witness  -A traceability list shall be provided when multiple heats/heat treatment batches are delivered in one shipment. -The content of the material certificate provided by the pipe manufacturer shall comply with the requirements in this specification and shall be reviewed and accepted by FMC and BP prior to delivery. |  | Quenched and tempered |  | T≤ 38.1 mm  (1 1/2") C Mn Si P S Mo Cr V Nb Ni Cu Al(total) Ti B Ca N As Sn Sb Pb Bi Nb+V+Ti V+Nb Cr+Mo Al/N | 0.12 0.80-1.60 0.10-0.45 0.015 0.003 0.30 0.35 0.060 0.05 0.10 0.25 0.015-0.055 0.03 0.0005 0.006 0.008 0.03 0.02 0.01 0.01 0.01 0.12 0.10 0.55 2:1min | T > 38.1 mm  (1 1/2") C Mn Si P S Mo Cr V Nb Ni Cu Al(total) Ti B Ca N As Sn Sb Pb Bi Nb+V+Ti V+Nb Cr+Mo Al/N | 0.12 0.80-1.65 0.10-0.45 0.015 0.003 0.35 0.35 0.080 0.05 0.20 0.25 0.015-0.055 0.03 0.0005 0.006 0.010 0.03 0.02 0.01 0.01 0.01 0.13 0.10 0.55 2:1min |  | T≤ 38.1 mm  (1 1/2"):  0.42     T > 38.1 mm (1 1/2"):  0.43 | T≤ 38.1 mm  (1 1/2"):  0,20 for WT≤ 19.1 mm  0.21 for 19.1 mm < WT≤ 38.1mm  T > 38.1 mm (1 1/2"):  0.23 | Min:  [NAME]: | 70  92 | 485  635 | Min:  [NAME]: | 82.7  110.2 | 570  760 | [NAME] 0.92 | Strip tensile:  Round bars: | Min 22  Min 18 |  | Transverse: -46 (-50)      Longitudinal: -46 (-50) | WT WT ≤ 38.1 mm(1-1/2") : WT > 38.1 mm(1-1/2") :   WT WT ≤ 38.1 mm(1-1/2") : WT > 38.1 mm(1-1/2") : | 50 37.5 25   60 45 30 | 40 30 20   45 33.75 22. | 250 HV10 |  |  |  | Mechanical test requirements:  -HIC/SWC Testing -SSC Testing -Crack Tip Opening              -Test Frequency -Retest Allowance -Displacement Testing  Hydrostatic test requirements.
M12003 | F |  | API 5L | X-52 | t<25mm | Seamless pipe | EN 10204 3.1 |  |  |  | C Mn P S V+Nb+Ti | [NAME] 0.28 max 1.40 [NAME] 0.030 [NAME] 0.030 [NAME] 0.15 |  |  | 0.45 |  | 0.24 |  | 52 | 359 | OD:  <20 inch  >20inch & t>9.5mm  >20 inch & t<9.5mm | 66   66   72 | 455   455   497 |  |  |  |  | DBI may contain Q-spec reference for sharpy requirements |  |  |  | 237 HB
M12003 | F |  | API 5L | X-52 | t<25mm | Welded pipe | EN 10204 3.1 |  |  |  | C Mn P S V+Nb+Ti | [NAME] 0.26 [NAME] 1.40 [NAME] 0.030 [NAME] 0.030 [NAME] 0.15 |  |  | 0.45 |  | 0.24 |  | 52 | 359 | OD:  <20 inch  >20inch & t>9.5mm  >20 inch & t<9.5mm | 66   66   72 | 455   455   497 |  |  |  |  | DBI may contain Q-spec reference for sharpy requirements |  |  |  | 237 HB
M12006 | G |  | API 5L ISO 3183 | X-65 Q L450 PSL 2 | t<25mm | Seamless and welded pipe | EN 10204 3.1 |  | The line pipe shall meet the heat treating requirements of the referenced API specifications. |  | C Si Mn P S V+Nb+Ti | [NAME] 0.18 max 0.45 max 1.70 [NAME] 0.025 max 0.015 [NAME] 0.15 |  |  | Q/M: 0.43 QS/MS: 0.42 |  | Q/M: 0.25 QS/MS: 0.22 |  | Min: 65.3  [NAME]: 87 | Min: 450  [NAME]: 600 | OD:  Min: <20 inch  >20inch & t>9.5mm  >20 inch & t<9.5mm  [NAME]: | 77.6   77.6   80   110,2 | 535   535   552   760 | 0.93 |  |  |  | DBI may contain Q-spec reference for sharpy requirements |  |  |  | 237 HBW
M12006 | G |  | API 5L ISO 3183 | X-65 M L450 PSL 2 | t<25mm | Welded pipe | EN 10204 3.1 |  | The line pipe shall meet the heat treating requirements of the referenced API specifications. |  | C Si Mn P S V+Nb+Ti | [NAME] 0.12 max 0.45 [NAME] 1.60 max 0.025 max 0.015 [NAME] 0.15 |  |  | Q/M: 0.43 QS/MS: 0.42 |  | Q/M: 0.25 QS/MS: 0.22 |  | Min: 65.3  [NAME]: 87 | Min: 450  [NAME]: 600 | OD:  Min: <20 inch  >20inch & t>9.5mm  >20 inch & t<9.5mm  [NAME]: | 77.6   77.6   80   110,2 | 535   535   552   760 | 0.93 |  |  |  | DBI may contain Q-spec reference for sharpy requirements |  |  |  | 237 HBW
M12006 | F |  | API 5L | X-65 | t<25mm | Seamless pipe | EN 10204 3.1 |  |  |  | C Mn P S V+Nb+Ti | [NAME] 0.28 max 1.40 [NAME] 0.030 [NAME] 0.030 [NAME] 0.15 |  |  | 0.45 |  |  |  | 65 | 448.5 | OD:  <20 inch  >20inch & t>9.5mm  >20 inch & t<9.5mm | 77   77   80 | 531   531   552 |  |  |  |  | DBI may contain Q-spec reference for sharpy requirements |  |  |  | 237 HB
M12006 | F |  | API 5L | X-65 | t<25mm | Welded pipe | EN 10204 3.1 |  |  |  | C Mn P S V+Nb+Ti | [NAME] 0.26 max 1.45 [NAME] 0.030 [NAME] 0.030 [NAME] 0.15 |  |  | 0.45 |  | 0.24 |  | 65 | 448.5 | OD:  <20 inch  >20inch & t>9.5mm  >20 inch & t<9.5mm | 77   77   80 | 531   531   552 |  |  |  |  | DBI may contain Q-spec reference for sharpy requirements |  |  |  | 237 HB
M12009 | E |  | API 5L | A | t<25mm | Seamless and welded pipe |  |  |  |  | C Mn P S Cu Ni Cr Mo | [NAME] 0.22 [NAME] 0.90 [NAME] 0.030 [NAME] 0.030 [NAME] 0.50 [NAME] 0.50 [NAME] 0.50 [NAME] 0.15 |  |  | 0.45 |  | 0.24 |  | 30 | 210 |  | 48 | 335 |  |  |  |  | DBI may contain Q-spec reference for sharpy requirements |  |  |  | 190 HB